MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS


 Ophelia Lewis
 1 years ago
 Views:
Transcription
1 MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS This paper provides a preliminary stress analysis of a carbon reinforced layered cylinder such as would be found in a yacht mast. The cylinder is subjected to a compressive load and both an analytical and numerical analysis of the resulting stress fields is obtained. Some conclusions are obtained regarding the failure mode for particular examples of such cylinders. Fiber reinforced materials are being increasingly used in specialist structures where high stiffness and low weight are of considerable importance. Examples of such specialist structures are turbine blades in jet engines and racing yacht masts. Carbon fiber reinforced materials provide many of the desirable characteristics required in such applications, but they also often display some highly undesirable and sometimes unexpected properties that cause problems in their use in specialist structures. For example, although carbon reinforced turbine blades may exhibit highly desirable characteristics in the radial direction, their properties in the transverse direction may limit their usefulness in this application. Similarly, in the area of racing yacht masts, it is possible to produce a carbon reinforced cylindrical mast which has the highly desirable properties of being relatively light and also has high stiffness in the axial direction along which the fibers are aligned. Unfortunately, when subjected to standard compressive loads in the axial direction, such masts are prone to fracture and splinter as the fibers 'pop out' of the resin which binds them together to form the reinforced composite. This undesirable property needs to be suitably countered if such masts are to be useful in racing yachts. One method of overcoming the problem is to wind layers of the fiber reinforced material around the mast both on the inside and outside in order to stop the axial fibers moving out of line. These inner and outer layers do 110tsignificantly improve the strength of the material in the axial direction and of course add to the weight of the mast. It is therefore important to minimize the inner and outer layers and to include no more material than is absolutely necessary to ensure the fibers in the central layer remain in line. The purpose of the preliminary analysis in this paper is to examine the relevant stress fields with a view to determining the minimum inner and outer reinforcing layers. To this end, the stress field in a layered fiber reinforced cylinder under a compressive load is considered. Both analytical and numerical
2 solutions to the problem are obtained. Both solutions have their limitations, but nevertheless provide some insight into the important features of the problem and also provide information regarding the likely failure mode for cylinders of this type. This analysis is specific to a threelayer tubular mast structure in the form of a circular cylinder which has thin walls relative to the mast radius. The mast is fabricated from a fiberreinforced material consisting of carbon fibers set in an epoxy resin. The middle lamina is oriented with the fibres in the mast direction, and the fibres in the inner and outer layers lie at 90 to the mast axis (i.e. they are purely circumferential). The load is taken to be axial, so no moment is supported and naturally the mast is straight. The fully anisotropic behaviour of the materials is incorporated in the linear regime, so the important consequences of these properties are fully evident in the final expressions. The ratio of the stresses in all members to the applied load is obtained for all the principal directions. How these ratios vary with the design of the laminae and the elastic properties of the material is then discussed. / superscript(o,m,i) width of inner layer width of middle layer width of outer layer radius of tube Young's modulus transverse to the fibres Young's modulus in longitudinal direction (i.e. along the fibres) Poisson's ratio coupling longitudinal strain to transverse strain Poisson's ratio coupling transverse to longitudinal strain normal stress in plane 1 to mast axis (compressive taken as positive) circumferential stress (tensile taken as positive) strain in radial direction strain in longitudinal direction refers to the outer, middle or inner layers
3 The conventions for stress are not totally consistent with those used in normal engineering practice, but the final formulae are quite simple and the sense of the stress is obvious in each particular case. The final design formulae are conventionindependent. Now for a material exhibiting transverse anisotropy (i.e. rotational symmetry about the fibre axis), the stiffness matrix has only five unknowns and hence the relation va Et V/t is easy to obtain (see for example Saada, 1974). The material properties relevant to this calculation are Et El tensile strength lt l tensile strength lt t compressive strength lt l compressive strength lt t 8 GPa 125 GPa 2090 MPa 64MPa Vlt ~ MPa 210 MPa El va ~ 0.02: very little Poisson coupling in this direction. Note that, typically, (a + b + c)/r ~ 0.02, so the tube is truly thin and use of the thin walled approximation in this analysis will only cause errors of the order of 1%. Also note that Ed Et ~ 15, so the tube is much stiffer longitudinally than transversely. 4. Theory for a simple longitudinal load applied to a straight mast, prior to bending in any way. If the composite is to deform as a whole under an applied load, then the strains of each component lamina must be the same in the radial and longitudinal directions. This is the central idea in the method of consistent deformations, also called the force method (see for example Popov, 1978). Now because of the symmetry of the stress field, the tube obviously remains circular, so any strain in the circumferential direction causes an identical strain in the radial direction. Thus, for example, we can write the total radial strain of the inner layer as (i) (i) (i) ltz (To Er = va E t + E 1
4 The first term is the coupling of the strain (ui i )/ Et) caused by the normal load to the circumferential direction via Vt/, and the second term is the direct circumferential strain caused by the circumferential stress u~i)/ E/. For the other two layers, the equivalent equations are (m) (m) f(m) uz u() r V/t E/ Et (0) (0) uz f(o) u() r Vt/ E t + E/. (3) (4) Now if we consider a small section of the complete laminate, subtended by a small angle do, then there is no net radial force on such a section (such as might come from internal pressure in boiler theory). Hence the radial projection of the circumferential forces must be zero, which for unit length gives (bu~m)+ au~i) + cu~o))sin do = 0 bu~m)+ au~i) + cu~o)= o. Hence, the laminae cannot all be in either tension or compression; it will soon become clear that the stress on the middle sheet is of the opposite sign to the stress on the inner and outer strapping. Using the same idea of considering a small section subtended by the angle do and applying radial force balance, it is easy to show that the interfacial stress in the radial direction on, say, the outer lamina, is given by u(mointerface) _ c u(o) r  r (). Similar relations can be written down for the other interfaces. Most importantly, these stresses are less than the circumferential stresses by approximately a factor of 50 (c/ r, b / r, a/ r), so it is realistic to neglect the Poisson induced strains in the circumferential and longitudinal directions caused by these stresses. This is the thin shell approximation. (0) (0) (0) u() uz f/ v/t+  E/ Et (m) (m) (m) u() uz f/ Vt/ (i) Et E/ (i) u() (i) uz f/ V/t E/ + E t ' (7) (8) (9)
5 IT the laminate is not to fail between the layers, then these strains must be equal. Equating the longitudinal strains (7,8,9) then gives two independent equations, and similarly two further equations are obtained by equating the radial strains (2,3,4). The force balance (5) provides a fifth equation. Now there are six unknown stresses, O'~o),O'~m),O'~i),O'}o),O'}m) and O'}i\ so it is now possible to express all of these stresses in terms of any single one of them. It is appropriate to choose the longitudinal stress O'~m) in the middle layer as the free parameter, since it bears the bulk of the load, as will be shown shortly. Solving ( ) fi h unk (0) (m) (i) (0) (i). equations 2,3,4,5,7,8,9 or t e nowns f O'(),O'(),O'(),O'z,O'z In terms 0 O'}m) gives: 1 1 Vlt  Vtl  VltVtl Et E, (a + c)(1  vl,) b a+c b(vit  Vtl) VltVtl Et E, (a + c)(1 vl,) b. { 2 E, (a + c)(1  VltVtl) } (0) (J) 1  vit + E b E O'z 0' z t t ( ) O'(m) = O'(m) = E, (a + c)(1  vl,) El 12 z z 1 VltVtl + E t b for the longitudinal stresses. Thus, for a compressive load, all the laminae are in compression in the zdirection, and the circumferential stress is tensile in the hoop layers but compressive in the middle layer. This is intuitively very plausible. The relation (12) is most interesting. Clearly if we make the material isotropic by putting Et = E, and thus V't = Vt/, then the right hand side of (12) becomes 1, as it should, and the layers would then be indistinguishable. Alternatively, if the mast was made of three loose concentric layers (i.e. with no stress coupling between the layers), then we would expect the above ratio to be (0) (i) E O'z O'z t (m)  (m)  E,' O'z O'z as is well known. This in fact is obtainable from (12) by sending VIt, Vtl + 0 to simulate 'loose coupling'. However when the layers are glued, the tension in the outer lamina (for a compressive load) 'pulls' these layers in along the mast axis, thereby increasing the fraction of the load taken by the middle lamina rather
6 slightly. For example, with the current mast proportions of b = 2a = 2c, the factor in curly braces in (12) is about However, for any realistic values of a, band c, the curly brace factor is not going to differ appreciably from 1, so this is not a significant fact. What is interesting is that these stress ratio formulae are symmetric in a and c. More precisely they are functions only of the sum a + c. This is probably due to the thin wall approximation  the basic algebraic system that has been set up is unable to distinguish inside from outside. This may not be such an unrealistic feature as might first be supposed. It is useful to show a simplified form of the stress ratios for the special case a = c (equal thickness inner and outer hoop layers). In this case the ratios are functions of only one free parameter, a/b, and may be written in the simple forms 0.33 < a/b a/b < a/b  a/b ) ( a/b ::; with the obvious inequalities on the right. Now if we compare these expressions to the ratios tensile strength IT[ compressive strength IT[ compressive strength lt t compressive strength IT[ it is immediately clear that, for all a/b, the inner and outer layers will not fail in longitudinal tension, nor in transverse compression, before the inner lamina fails in longitudinal compression. Similarly the middle layer will not fail in transverse compression before it fails in longitudinal compression. Interestingly, these formulae indicate that even very thin hoop layers (a/b ~ 0) are at about 27% of their tensile strength, and, at worst, 52% of their transverse compressive strength, at the point where the inner layer fails in longitudinal compression.
7 A numerical analysis relevant to the problem specified in Section 2 was carried out using using the finite element package MSC/NASTRAN with bilinear quad shell elements (membrane plus bending). The analysis was based on classical bending theory. A linear static analysis was considered to examine material failure prior to buckling. Also a linear buckling analysis (eigenvalue) and a geometric nonlinear analysis (without imperfections) for local buckling of a thin shell was considered to determine the failure load due to buckling (see figures 2, 3 and 4). The results obtained are summarized in figure 1 which provides the failure load for a cylinder under compression with the total width of the cylinder wall being 1 millimeter and the percentage of the total material forming the inner and outer layers given as percentage hoop reinforcment in the graph. ~ '" 180 ~ 160 :: (> <) ~~.~ A l:: Material failure  max strain failure theory ~'local buckling  eigenvalue analysis.. l::... local buckling  geometric nonlinear analysis 100 o Figure 1: Material failure and local buckling for a carbon/epoxy Wall thickness is 1 mid. composite mast. The numerical results indicate that buckling of the mast will occur before compressive failure in the middle layer. Furthermore the results show that for a mast of 1 millimeter thickness the load at which buckling occurs is maximised by having at least 15% of the mast distributed equally in the inner and outer layers. Since it is appropriate to have as much as possible of the mast in the middle layer to support the compressive load these results suggest no more than 15% of the mast should be distributed in the inner and outer layers.
8 Local buckling is not sensitive to LID ratio
9 ...: ITr. t ~ N 10:;:.r ~ ~ I.'( ~ ~6 ~ '\ N '\:: 4I: 'J Figure 4: Linear buckling: eigenvalue analysis. (a) Compression, lowest eigenvalue. (b) Compression, higher mode. (c) Compression plus bending, lowest eigenvalue. If the possibility of buckling is ignored then the conclusion from the analysis in Sections 14 would be to make the inner and outer hoop layers as small
10 as is convenient. This is because the area of the middle lamina would need to be increased as much as possible in order to reduce the compressive stress for a given load and mast weight. This seems to be in accord with a mast constructor's observation that 'only a layer of sticky tape is needed to keep the layers in'. Accordingly, if a/ b is small, it is possible to naively obtain an upper bound for the stress in the middle lamina from equation (16), 00(m)! < IPI 1 z  21l"T(0.113a+ b)' assuming an applied compressive load P. This can be rearranged restriction to give the 0.113a + b > IPI. (20) 21l"TO'I compressive strength' but this formula is likely to grossly underestimate the required thickness since, as is clear from the numerical analysis, buckling is very likely to occur prior to pure compressive failure. Unfortunately, there are no simple analytical formulae which give a clear indication as to how the stresses vary in bending or local buckling. However, buckling formulae are usually sensitive only to elastic constants (e.g. the Euler formula or the beercan formula), so the critical buckling load of this composite is likely to be given by a complicated function of the anisotropic elastic constants only. It is difficult to estimate how this will vary with a/b. Nevertheless, the simple theory given above does give a reasonably accurate idea of how the stresses are distributed prior to failure, and thus may be of some use in the construction of yacht masts. It seems likely that, given the slenderness ratios and rigging supports used in practice, the material will fail in local buckling or longitudinal compression well before the Euler load. But consider the beercan formula for an isotropic thin cylinder of thickness h and radius T (see Timoshenko, 1961): Eh O'er = J ( 2)' T 31v If h/t ~ 1, then the buckling stress O'er is usually well below the compressive strength. Unfortunately, in the case of these masts, h/t is not especially small, so the local buckling strength is likely to be of the same order as the compressive strength. Another possible problem is that the beercan failure wavelengths might be quite large, so an experiment or finiteelement calculation might have to use a fairly long cylinder to avoid any finitelength dependence of the critical stress. The simple isotropic formulae predict about a 30 millimeter wavelength for a 92 millimeter diameter mast of thickness 1 millimeter.
11 It seems likely that a full finite element calculation has to be done to satisfactorily analyse the problem. And given the size of the 'parameter space' (the range of possible loads, afb, etc.) through which such a calculation would have to search, perhaps some restrictive decision would need to be made about the type of loads considered. The direct axial load may be a good starting point, since it can be directly compared with the preceding theory; the expressions given above are probably a good check on the finite element calculation prior to buckling. Secondly, from the simple statics of the rigging etc., it should be possible to find that part of the mast subject to the maximum moment, and use this moment plus the axial load as the load conditions in another finite element computation. Then it would be appropriate to try to maximise the load as a function of afb, as was attempted at the MISG. Naturally the finite element result would have to be meshindependent, and free of any finite length artifacts. The moderators ( David Clements and Aaron Blicblau) would like to thank Rob Denney, owner of Carbon Design, for presenting this problem. They would also like to thank James Gunning for his contribution to the analytical analysis and David Rees for his contribution to the numerical analysis. The assistance of Barrie Fraser, Vincent Hart, Walter Neumann, John Sader, Derek Wilson and Graham Wood is gratefully acknowledged. E.P. Popov, Mechanics of materials, 2nd Ed. (PrenticeHall, Englewood Cliffs, NJ,1978). A.S. Saada, Elasticity theory and applications (Pergamon Press, New York, 1974). S. Timoshenko, Theory of elastic stability, 2nd Ed. (McGrawHill, New York, 1961).
Module 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationAnalysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method
Analysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method V.M.F. Nascimento Departameto de ngenharia Mecânica TM, UFF, Rio de Janeiro
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More information8. Combined Loadings
CHAPTER OBJECTIVES qanalyze the stress developed in thinwalled pressure vessels qreview the stress analysis developed in previous chapters regarding axial load, torsion, bending and shear qdiscuss the
More informationEngineering Mechanics Department of Mechanical Engineering Dr. G. Saravana Kumar Indian Institute of Technology, Guwahati
Engineering Mechanics Department of Mechanical Engineering Dr. G. Saravana Kumar Indian Institute of Technology, Guwahati Module 3 Lecture 6 Internal Forces Today, we will see analysis of structures part
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationChapter 5 Torsion STRUCTURAL MECHANICS: CE203. Notes are based on Mechanics of Materials: by R. C. Hibbeler, 7th Edition, Pearson
STRUCTURAL MECHANICS: CE203 Chapter 5 Torsion Notes are based on Mechanics of Materials: by R. C. Hibbeler, 7th Edition, Pearson Dr B. Achour & Dr Eng. K. Elkashif Civil Engineering Department, University
More informationDesign of Automobile Driveshaft using Carbon/Epoxy and Kevlar/Epoxy Composites
American Journal of Engineering Research (AJER) eissn : 23200847 pissn : 23200936 Volume02, Issue10, pp173179 www.ajer.org Research Paper Open Access Design of Automobile Driveshaft using Carbon/Epoxy
More information(laod No \' V,R A " FI 1 4, <4. ELASTIC STABILITY Of CYLINDRICAL SANDWICH SHELLS UNDER AXIAL AND LATERAL LOAD. July 1955
ELASTIC STABILITY Of CYLIDRICAL SADWICH SHELLS UDER AXIAL AD LATERAL LOAD (laod o. 1852 July 1955 This Report is One of a Series Issued ha Cooperation with the AC23 PAEL O SADWICH COSTRUCTIO of the Departments
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationMechanical Design in Optical Engineering
OPTI Buckling Buckling and Stability: As we learned in the previous lectures, structures may fail in a variety of ways, depending on the materials, load and support conditions. We had two primary concerns:
More informationBuckling Resistance Assessment of a Slender Cylindrical Shell Axially Compressed
Mechanics and Mechanical Engineering Vol. 14, No. 2 (2010) 309 316 c Technical University of Lodz Buckling Resistance Assessment of a Slender Cylindrical Shell Axially Compressed Jakub Marcinowski Institute
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationDeflections and Strains in Cracked Shafts Due to Rotating Loads: A Numerical and Experimental Analysis
International Journal of Rotating Machinery, 9: 303 311, 2003 Copyright c Taylor & Francis Inc. ISSN: 1023621X DOI: 10.1080/10236210390147416 Deflections and Strains in Cracked Shafts Due to Rotating
More informationCIVL222 STRENGTH OF MATERIALS. Chapter 6. Torsion
CIVL222 STRENGTH OF MATERIALS Chapter 6 Torsion Definition Torque is a moment that tends to twist a member about its longitudinal axis. Slender members subjected to a twisting load are said to be in torsion.
More informationDeflections and Strains in Cracked Shafts due to Rotating Loads: A Numerical and Experimental Analysis
Rotating Machinery, 10(4): 283 291, 2004 Copyright c Taylor & Francis Inc. ISSN: 1023621X print / 15423034 online DOI: 10.1080/10236210490447728 Deflections and Strains in Cracked Shafts due to Rotating
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More informationLecture 7, Foams, 3.054
Lecture 7, Foams, 3.054 Opencell foams StressStrain curve: deformation and failure mechanisms Compression  3 regimes  linear elastic  bending  stress plateau  cell collapse by buckling yielding
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationDiscontinuous Distributions in Mechanics of Materials
Discontinuous Distributions in Mechanics of Materials J.E. Akin, Rice University 1. Introduction The study of the mechanics of materials continues to change slowly. The student needs to learn about software
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationUnit III Theory of columns. Dr.P.Venkateswara Rao, Associate Professor, Dept. of Civil Engg., SVCE, Sriperumbudir
Unit III Theory of columns 1 Unit III Theory of Columns References: Punmia B.C.,"Theory of Structures" (SMTS) Vol II, Laxmi Publishing Pvt Ltd, New Delhi 2004. Rattan.S.S., "Strength of Materials", Tata
More informationLINEAR AND NONLINEAR SHELL THEORY. Contents
LINEAR AND NONLINEAR SHELL THEORY Contents Straindisplacement relations for nonlinear shell theory Approximate straindisplacement relations: Linear theory Small strain theory Small strains & moderate
More informationComparison of Euler Theory with Experiment results
Comparison of Euler Theory with Experiment results Limitations of Euler's Theory : In practice the ideal conditions are never [ i.e. the strut is initially straight and the end load being applied axially
More informationMars Ascent Vehicle Hybrid Motor Structural Analysis
Mars Ascent Vehicle Hybrid Motor Structural Analysis MSFC  James Luce ER41 (Summer intern program) NASA Sensitive But Unclassified 1 Background: the MAV MAV: Mars Ascent Vehicle (MAV) is a small rocket
More informationCivil Engineering Design (1) Design of Reinforced Concrete Columns 2006/7
Civil Engineering Design (1) Design of Reinforced Concrete Columns 2006/7 Dr. Colin Caprani, Chartered Engineer 1 Contents 1. Introduction... 3 1.1 Background... 3 1.2 Failure Modes... 5 1.3 Design Aspects...
More informationINSTITUTE OF AERONAUTICAL ENGINEERING (Autonomous) Dundigal, Hyderabad
INSTITUTE OF AERONAUTICAL ENGINEERING (Autonomous) Dundigal, Hyderabad 00 04 CIVIL ENGINEERING QUESTION BANK Course Name : STRENGTH OF MATERIALS II Course Code : A404 Class : II B. Tech II Semester Section
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationUNIT I SIMPLE STRESSES AND STRAINS
Subject with Code : SM1(15A01303) Year & Sem: IIB.Tech & ISem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationLecture #10: Anisotropic plasticity Crashworthiness Basics of shell elements
Lecture #10: 1510735: Dynamic behavior of materials and structures Anisotropic plasticity Crashworthiness Basics of shell elements by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering,
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More information7.5 Elastic Buckling Columns and Buckling
7.5 Elastic Buckling The initial theory of the buckling of columns was worked out by Euler in 1757, a nice example of a theory preceding the application, the application mainly being for the later invented
More informationBUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationInitial Stress Calculations
Initial Stress Calculations The following are the initial hand stress calculations conducted during the early stages of the design process. Therefore, some of the material properties as well as dimensions
More informationMachine Direction Strength Theory of Corrugated Fiberboard
Thomas J. Urbanik 1 Machine Direction Strength Theory of Corrugated Fiberboard REFERENCE: Urbanik.T.J., Machine Direction Strength Theory of Corrugated Fiberboard, Journal of Composites Technology & Research,
More informationSERVICEABILITY OF BEAMS AND ONEWAY SLABS
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONEWAY SLABS A. J. Clark School of Engineering Department of Civil
More informationFinite Element Modelling with Plastic Hinges
01/02/2016 Marco Donà Finite Element Modelling with Plastic Hinges 1 Plastic hinge approach A plastic hinge represents a concentrated postyield behaviour in one or more degrees of freedom. Hinges only
More informationLATERAL STABILITY OF DEEP BEAMS WITH SHEARBEAM SUPPORT
U. FOREST SERVICE RESEARCH PAPER FPL 43 OCTOBER U. S. DEPARTMENT OF AGRICULTURE FOREST SERVICE FOREST PRODUCTS LABORATORY MADISON, WIS. LATERAL STABILITY OF DEEP BEAMS WITH SHEARBEAM SUPPORT The FOREST
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationModeling of FiberReinforced Membrane Materials Daniel Balzani. (Acknowledgement: Anna Zahn) Tasks Week 2 Winter term 2014
Institute of echanics and Shell Structures Faculty Civil Engineering Chair of echanics odeling of FiberReinforced embrane aterials OOC@TU9 Daniel Balani (Acknowledgement: Anna Zahn Tasks Week 2 Winter
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationSDLS505  Buckling of a cylindrical envelope under external pressure
Titre : SDLS505  Flambement d une enveloppe cylindrique s[...] Date : 03/05/2016 Page : 1/10 SDLS505  Buckling of a cylindrical envelope under external pressure Summary: This test represents a calculation
More informationTask 1  Material Testing of Bionax Pipe and Joints
Task 1  Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 6045348631 Fax: 6045347616
More informationNow we are going to use our free body analysis to look at Beam Bending (W3L1) Problems 17, F2002Q1, F2003Q1c
Now we are going to use our free body analysis to look at Beam Bending (WL1) Problems 17, F00Q1, F00Q1c One of the most useful applications of the free body analysis method is to be able to derive equations
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationBUCKLING STRENGTH ANALYSIS OF BARS AND FRAMES, AND SPHERICAL SHELLS
CLASSIFICATION NOTES No. 30.1 BUCKLING STRENGTH ANALYSIS OF BARS AND FRAMES, AND SPHERICAL SHELLS APRIL 004 Veritasveien 1, NO13 Høvik, Norway Tel.: +47 67 57 99 00 Fax: +47 67 57 99 11 FOREWORD is an
More informationOnly for Reference Page 1 of 18
Only for Reference www.civilpddc2013.weebly.com Page 1 of 18 Seat No.: Enrolment No. GUJARAT TECHNOLOGICAL UNIVERSITY PDDC  SEMESTER II EXAMINATION WINTER 2013 Subject Code: X20603 Date: 26122013 Subject
More informationSemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials
International Journal of Composite Materials 2017, 7(3): 103114 DOI: 10.5923/j.cmaterials.20170703.03 SemiMembrane and Effective Length Theory of Hybrid Anisotropic Materials S. W. Chung 1,*, G. S. Ju
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationNumerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints
THEORETICAL & APPLIED MECHANICS LETTERS 1, 041005 (2011) Numerical investigation on the position of holes for reducing stress concentration in composite plates with bolted and riveted joints M. R. Khoshravan,
More informationNew Representation of Bearings in LSDYNA
13 th International LSDYNA Users Conference Session: Aerospace New Representation of Bearings in LSDYNA Kelly S. Carney Samuel A. Howard NASA Glenn Research Center, Cleveland, OH 44135 Brad A. Miller
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationSTRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS STRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK Md. S. Uddin 1*, E. V. Morozov 1 and K. Shankar 1 1 School of Engineering and Information
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationTRESS  STRAIN RELATIONS
TRESS  STRAIN RELATIONS Stress Strain Relations: Hook's law, states that within the elastic limits the stress is proportional to t is impossible to describe the entire stress strain curve with simple
More informationComputational models of diamond anvil cell compression
UDC 519.6 Computational models of diamond anvil cell compression A. I. Kondrat yev Independent Researcher, 5944 St. Alban Road, Pensacola, Florida 32503, USA Abstract. Diamond anvil cells (DAC) are extensively
More informationMECHANICS LAB AM 317 EXP 5 COLUMN BEHAVIOR BUCKLING
MECHANICS LAB AM 317 EX 5 COLUMN BEHAVIOR BUCKLING I. OBJECTIVES I.1 To determine the effect the slenderness ratio has on the load carrying capacity of columns of varying lengths. I. To observe short,
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More informationStress Analysis on Bulkhead Model for BWB Heavy Lifter Passenger Aircraft
The International Journal Of Engineering And Science (IJES) Volume 3 Issue 01 Pages 3843 014 ISSN (e): 319 1813 ISSN (p): 319 1805 Stress Analysis on Bulkhead Model for BWB Heavy Lifter Passenger Aircraft
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationMassachusetts Institute of Technology 22.68J/2.64J Superconducting Magnets. February 27, Lecture #4 Magnetic Forces and Stresses
Massachusetts Institute of Technology.68J/.64J Superconducting Magnets February 7, 003 Lecture #4 Magnetic Forces and Stresses 1 Forces For a solenoid, energy stored in the magnetic field acts equivalent
More informationMECHANICS OF SOLIDS Credit Hours: 6
MECHANICS OF SOLIDS Credit Hours: 6 Teaching Scheme Theory Tutorials Practical Total Credit Hours/week 4 0 6 6 Marks 00 0 50 50 6 A. Objective of the Course: Objectives of introducing this subject at second
More informationTHEME IS FIRST OCCURANCE OF YIELDING THE LIMIT?
CIE309 : PLASTICITY THEME IS FIRST OCCURANCE OF YIELDING THE LIMIT? M M  N N + + σ = σ = + f f BENDING EXTENSION Ir J.W. Welleman page nr 0 kn Normal conditions during the life time WHAT HAPPENS DUE TO
More informationMECH 344/X Machine Element Design
1 MECH 344/X Machine Element Design Time: M 14:4517:30 Lecture 2 Contents of today's lecture Introduction to Static Stresses Axial, Shear and Torsional Loading Bending in Straight and Curved Beams Transverse
More informationSteam Generator Tubing Inspection
Steam Generator Tubing Inspection Analytical Determination of Critical Flaw Dimensions in Steam Generator Tubing I. Kadenko, N. Sakhno, R. Yermolenko, Nondestructive Examination Training and Certification
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationBUCKLING AND POSTBUCKLING ANALYSIS OF SHELLS UNDER QUASISTATIC AND DYNAMIC LOADS
BUCKLING AND POSTBUCKLING ANALYSIS OF SHELLS UNDER QUASISTATIC AND DYNAMIC LOADS R. Degenhardt, H. Klein, A. Kling, H. Temmen, R. Zimmermann DLR Institute of Structural Mechanics Lilienthalplatz 7, 388
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationDesign Principles of Superconducting Magnets
1 Design Principles of Superconducting Magnets Aki Korpela Tampere University of Technology DESIGN PRINCIPLES OF SUPERCONDUCTING MAGNETS 2 Content of the presentation Background Shortsample measurement
More informationInternational Conference on Mechanics and Civil Engineering (ICMCE 2014)
International Conference on Mechanics and Civil Engineering (ICMCE 2014) Parametric Design and Experimental Study for Weak Area Structure of Circle Composite Fragile Cover Ran CAO 1,a, GuangMing ZHOU
More information